Bisque, bisquit firing
Generally, bisque firing refers to the practice of prefiring ware without glaze to make it impervious to water, resistant to damage during handling and absorbent for glazing. The porosity of the bisque (generally more than 15%) makes it an ideal medium to absorb water from the glaze suspension and hold it in place, it is typical for the glaze to dry sufficiently for handling in just a few seconds. The temperature of the bisque firing can be adjusted to tune the degree of porosity, and therefore the glazing characteristics. Bisquit should be fired as high as possible to burn away all carbonaceous matter, yet low enough to provide enough absorbency to make glaze application easy. Less porous ware can be successfully glazed by reducing water content of the glaze suspension, heating the ware before immersion in the glaze, additions of binders or flocculants, applying a thinner layer, etc.
A dried terra cotta mug on the left, bisque fired to cone 06 on the right
These were fired to cone 06, about 1800F. Of course, there is normally some shrinkage so the bisque piece would be a little smaller. Even though the matrix is very porous and is under developed, the iron in the body is already beginning to impose its color.
Why would you bisque fire glazed ware? For transport for glaze firing.
These are high temperature stoneware mugs that have been bisque fired, glazed and then bisque fired again to cone 02. This is done so they can be handled without damage (they are being shipped to another location for firing to cone 10R). The glaze is quite durable at this point and would be difficult to damage.
How much does the size of a piece change when it is bisque fired? Glaze fired?
Three mugs. Dry. Bisque fired. Glaze fired. Notice the shrinkage at each stage (these were the same size in the dry state).
At what temperature do cone 6 glazes seal off the surface of the body?
These are 10 gram balls of four different common cone 6 clear glazes. I fired them to 1800F (bisque temperature) to see how dense they would be. Why? To answer this question: If the gases of decomposing lignite have not been fully expelled from the clay body during bisque, then could a glaze densify enough to seal the surface from that temperature up? The answer appear to be yes. I measured the porosity of these (weighing, soaking, weighing again): G2934 - 21%. G2926B - 0%. G2916F - 8%. G1215U - 2%. The implications: Glaze pinholes in improperly bisqued ware.
Lignite can be big trouble
Example of the lignite particles in a fireclay (Pine Lake) that have been exposed on the rim of a vessel after sponging. This is a coarse clay, but if it were incorporated into a recipe of a stoneware, glaze pinholing would be likey.
Oversize particles in a typical manufactured porcelain body
Example of the oversize particles from a 100 gram wet sieve analysis test of a powdered sample of a porcelain body made from North American refined materials. Although these materials are sold as 200 mesh, that designation does not mean that there are no particles coarser than 200 mesh. Here there are significant numbers of particles on the 100 and even 70 mesh screens. These contain some darker particles that could produce fired specks (if they are iron and not lignite); that goodness in this case they do not. Oversize particle is a fact of life in bodies made from refined materials and used by potters and hobbyists. Industrial manufacturers (e.g. tile, tableware, sanitaryware) commonly process the materials further, slurrying them and screening or ball milling; this is done to guarantee defect-free glazed surfaces.
Lignite contamination in manufactured porcelain bodies
These particles contaminating particles are exposed on the rim of a bisque fired mug. The liqnite ones have burned away but the iron particle is still there (and will produce a speck in the glaze). Remnants of the lignite remain inside the matrix and can pinhole glazes. Since ball clays are air floated (a stream of air takes away the lighter particles and the heavier ones recycle for regrinding) it seems that contamination like this would be impossible. But the equipment requires vigilance for correct operation, especially when there is pressure to maximize production. Ores in Tennessee are higher in coal than those in Kentucky. North American clay body manufacturers who confront ball clay suppliers with this contamination find that ceramic applications have become a very small part of the total ball clay market, complaints are not taken with the same seriousness as in the past.
How much does clay shrink when bisque fired?
Not much. These mugs were exactly the same height before a bisque firing to cone 06. The clay is a porcelain made from kaolin, feldspar and silica.
Do not glaze bisque ware when it is too wet
These mugs are quite thin walled. A glaze has just been applied to the inside. Notice how it has water logged the bisque (you can see the contrast at the base, where the clay is a little thicker and has not changed color yet). Although there may be enough absorbency that a glaze could be applied now, it would still not be a good idea because it would completely waterlog the piece and result in a very long drying time. This is bad, not only because of process logistics, but also because slow drying glazes almost always crack and lift from the bisque (causing crawling).
Can you bisque fire at cone 02? Yes. But why? How?
The buff stoneware mug on the right was bisque fired at cone 02, the one on the left at cone 06. The cone 02 mug was immersed in the clear glaze for 1 second and allowed to dry. The other was glazed on the inside first, allowed to dry, then glazed on the outside with a 1 second dip. Of course, the cone 02 one took longer to dry. In spite of this, the glaze is thicker and more even on the one bisque fired to cone 02. How is the possible? The secret is the thixotropy of the glaze. When that is right, a one second dip will give the same thickness and evenness whether dry or bisque, 06 or 02. Why bisque fire to cone 02? To get a glazed surface free of pinholes on some stoneware clays.
Bisque temperature can be lower than you think
These bowls are made from a talc:ball clay mix, they are used for calcining Alberta and Ravenscrag Slips (each holds about one pound of powder). The one on the right was bisque fired to cone 04 (about 1950F). The one on the left was fired to only 1000F (540C, barely red heat), yet it is sintered and is impervious to water (strong enough to use for our calcining operations). That means that there is potential, in many production situations, to bisque a lot lower (and save energy). Primitive cultures made all their ware a very low temperatures. Tin foil melts at 660C (1220F) yet can be used on campfires for cooking (so the temperatures of primitive wares would have been low indeed).
Out Bound Links
In Bound Links